Research Article  Open Access
Lamia Bourja, Bahcine Bakiz, Abdeljalil Benlhachemi, Mohamed Ezahri, Sylvie Villain, Claude Favotto, JeanRaymond Gavarri, "Electrical Properties of a CeO_{2} Mix System Elaborated at 600°C", Advances in Materials Science and Engineering, vol. 2012, Article ID 452383, 11 pages, 2012. https://doi.org/10.1155/2012/452383
Electrical Properties of a CeO_{2}Mix System Elaborated at 600^{∘}C
Abstract
The electrical conduction of a series of polycristalline [(1−x)CeO_{2}·x/2Bi_{2}O_{3}] samples has been analyzed using electrical impedance spectroscopy, in the temperature range 25 to C. Samples have been prepared via a coprecipitation route followed by a pyrolysis process at C. For compositions , Ce_{1−x}Bi_{x}O_{2−x/2} solid solutions, with fluorite cubic structure, are obtained. In the composition range , the system is biphasic with coexistence of cubic and tetragonal structures. To interpret the Nyquist representations of electrical analyses, various impedance models including constant phase elements and Warburg impedances have been used. In the biphasic range (), the conductivity variation might be related to the increasing fraction of two tetragonal β′ and βBi_{2}O_{3} phases. The stabilization of the tetragonal phase coexisting with substituted ceria close to composition is associated with a high conduction of the mix system CeO_{2}Bi_{2}O_{3}.
1. Introduction
Recently, in a structural analysis [1] of the polycrystalline system ( with , elaborated at 600°C, we have observed the partial stabilization of two tetragonal varieties of Bi_{2}O_{3} oxide coexisting with a substituted ceria phase. Presently, we analyze the electrical properties of this CeO_{2}Bi_{2}O_{3} system as a function of composition x and at various temperatures.
Cerium dioxide (ceria) is well known for its applications as ceramic pigments, solid electrolyte in fuel cells, and catalyst in automotive gas converters [2–9]. Ceria presents mixed ionic and electronic conductivity [10, 11]. In a previous work on the neodymiumsubstituted phase Ce_{(1x)}Nd_{x}O_{2x/2} [12], we showed that the conductivity increased with composition x up to a value of in the cubic lattice. Other studies have shown a similar effect with other elements: europium [13], iron [14], gadolinium [15], samarium [16], and terbium [17].
In 1937, Sillen [18] published the first study on the complex polymorphs of Bi_{2}O_{3} using Xray diffraction (XRD) analysis. Four polymorph phases were proposed: (i) the αBi_{2}O_{3} monoclinic phase, stable at low temperatures; (ii) the δBi_{2}O_{3} facecentered cubic phase, stable at high temperatures (above 729°C); (iii) the two intermediate β and γBi_{2}O_{3} phases that can stabilize with tetragonal and bodycentered cubic (bcc) lattices, respectively, depending on the cooling mode. An additional polymorph was also observed by the authors [19]: a Bi_{2}O_{3} tetragonal modification that should be a superstructure of the β phase. During cooling of the hightemperature cubic δBi_{2}O_{3} phase to T = 650°C, this δ phase can transform into the βBi_{2}O_{3 }tetragonal modification. However, below T = 640°C, this δ phase can transform into the γ (body centered cubic) modification. If this γ phase is formed, it transforms into the αBi_{2}O_{3} monoclinic phase close to 500°C. However, if the β phase is formed, it transforms into the α phase close to 330°C [20–22].
Several studies on the electrical properties of Bi_{2}O_{3} [22–28] have shown that conduction is mainly ionic above 500°C. According to the authors, this ionic conduction should be favored by the existence of vacancies or empty spaces in the hightemperature structure that allows fast mobility of the oxygen ions in the lattice. Chemical units noted as Bi_{4}O_{6}□_{2} are organized into a structure that is closely related to that of fluorite (basic A_{4}O_{8} units). Both cerium and bismuth oxides should exhibit similar crystal packing in which the oxygen vacancies are associated with the Bi^{3+} ions: the ceria chemical unit Ce_{4}O_{8} might be converted into the Bi_{4}O_{6}□_{2} chemical unit in which the Bi^{3+} ions substitute for the Ce^{4+} ions and oxygen vacancies substitute for the oxygen atoms. Some authors have proposed that the presence of lone pairs could play a role in the observed phase transition α (monoclinic) → δ (cubic) at 729°C and in the measured high conductivity.
The substituted phases Ce_{1x }Bi_{x}O_{2δ} have already been studied by Dikmen et al. [29], and the solubility limit was found to be . However, very few data are available on the section of the phase diagram with .
It is interesting to note that the authors Chen and Eysel [30] studied the composite system CeO_{2}Bi_{2}O_{3} in the composition range to and observed that the metastable β phase was stabilized by the presence of the ceria phase. They suggest that this stabilization should be provoked by a certain proximity effect. They considered that this stabilization was not due to any insertion of cerium ions in the Bi_{2}O_{3} lattice.
Recently, using hydrothermal route, Sardar et al. [31] synthesized phases with having cerialike fluorite structure with local distortions.
In our previous work [1], we observed at least three domains for these samples obtained at 600°C. In agreement with literature results, a first solidsolution domain was observed for , with a limiting composition close to . Surprisingly, we also found evidence for a second biphasic system with , which should be constituted of the limit phase with coexisting with a tetragonal phase quite similar to the Bi_{2}O_{3} phase. A third biphasic system was also observed for , with coexistence of the tetragonal βBi_{2}O_{3} phase and the monoclinic αBi_{2}O_{3} phase, which is stable at low temperatures. The tetragonal polymorph (lattice parameters: nm; nm) is a superstructure of the β phase (lattice parameters: nm; nm). In the past, both phases were considered to be metastable varieties of pure Bi_{2}O_{3} oxide. In our specific case, the modification ↔β depending on composition should result from orderingdisordering of cerium defects in the lattice: ordering ( phase stabilization) should require sufficient fraction of cerium atoms in the lattice, while disordering (β phase stabilization) should be due to insufficient fraction of cerium atoms in the lattice. Finally, for , we obtained a stable monoclinic structure (lattice parameters: nm; nm; nm; β = 112.95°). In our study, we also observed typical variations in the volumes of the chemical units A_{4}O_{8} (Ce_{4}O_{8} for the ceria structure and Bi_{4}O_{6}□_{2} for the and β phases). For compositions , the volume increase is directly due to the increased Bi^{3+} fraction. For compositions , the volume increase can be interpreted in terms of the increasing fraction of metastable phase Bi_{2}O_{3} coupled with a decreasing fraction of defects in the Bi_{2}O_{3} lattice. For compositions , the volume reaches a stabilized value due to the very weak concentration of cerium defects. The large decrease in volume for should be due to the formation of the more compact monoclinic αBi_{2}O_{3} structure. These variations are reported on Figure 1 (see [1]).
At present, we are trying to elucidate the role of the bismuth composition on the ionic conduction of this mixed system. Such composite systems could present a very high interest in the case of electrolytic applications.
2. Experimental Section
2.1. Sample Elaboration
Samples of bismuth/ceriumbased precursors having the composition ( with were prepared via a precipitation route [32–36] using appropriate quantities of cerium(III) nitrate hexahydrate, Ce(NO_{3})_{3}·6H_{2}O (purity 99.5%), and bismuth(III) nitrate pentahydrate Bi(NO_{3})_{3}·5H_{2}O (purity ≥ 98%). Each nitrate was separately dissolved in suitable volumes of distilled water. The two nitrate solutions were mixed and stirred for two hours at room temperature. Ammonium hydroxide (NH_{4}OH) was added to the mixture to adjust the pH to 10. The resulting precipitate was filtered, washed with distilled water to remove residual , and dried at 80°C. Finally, the precursor powder was heated in air at 600°C for 6 hours. We obtained eleven samples of compositions , 0.10, 0.20, 0.30, 0.40, 0.50, 0.60, 0.70, 0.80, 0.90, and 1.00. In Table 1, we report the experimental and calculated densities, the apparent porosities (), and grain sizes [1]. The calculated density is obtained from a theoretical evaluation taking into account a mean molar mass (A_{4}O_{8} formula depending on composition ) and a mean volume of chemical unit A_{4}O_{8} (see Figure 1) depending on composition , determined from the crystal structure of each phase. In the mix system where substituted ceria and tetragonal phases ( or β) coexist, the phase ratio has been calculated using the classical lever rule.
 
Note: (g·cm^{−3}) = m/V; . 
2.2. Electrical Analyses
The electrical study was performed using an electrical impedance spectrometer SOLARTRON SI 1260 coupled to an electrical cell operating under air and in the temperature range from 25 to 750°C. The samples were cylindrical pellets (diameter mm, thickness 2 ± 0.05 mm) initially compacted at 5 kbar under ambient conditions. Each apparent density was calculated and compared with the theoretical value to determine the fraction of cavities. The pellets were placed between two cylindrical platinum electrodes in a specific cell. A constant pressure was applied to the electrodes via rings. The cell was placed in a furnace operating at up to 750°C.
The electrical analyses were carried out in the frequency range (ω = 2πν) 10^{−1} to 10^{7} Hz, with an alternating current associated with a maximum voltage of 0.1 V. Samples were stabilized for 15 minutes at a fixed temperature. The recording time for the frequency range was of 15 minutes. To ensure thermal stabilization of pellets, each sample was subjected to three successive measuring cycles (with one temperature rise and drop for each cycle). The final impedance data were chosen during heating mode of the third cycles, as being representative of stabilized samples (these data were identical to those of the second cycle).
The impedances ( and being, resp., the real and imaginary components) were represented using Nyquist plots (). The software Zview [37] was used to fit the impedances of specific electrical circuits to the Nyquist experimental data (Nyquist representations). The equivalent circuits associated with each sample were generally based on parallel RC circuits; constantphase elements (CPE) having the form (CPE) = were systematically tested. At low temperature (°C), the impedance of such parallel RC circuits is generally expressed as a function of frequency ω as follows: In these expressions, is the resistance (associated with the intersection of the Nyquist circle with real axis), the CPE term is expressed in Ω^{−1}·Hz^{n}, the frequency ω is expressed in Hz, is the exponent describing the deviation from the ideal capacitor model and is characteristic of the CPE model.
In the case of high temperature results (°C), it has been necessary to use a specific modified Warburg model [38–42] having the following form: with as a specific resistance (in Ω), as a specific term depending on diffusion mechanisms, related to the electrode or interface responses (see the appendix), and being an exponent characteristic of the diffusion process coupled with the sample heterogeneity. In the case of pure Warburg diffusion mechanism, this value should be equal to 1/2.
Three circuits placed in series were systematically tested for grain core, grain interface, and electrode contributions. At high temperature, the high frequency impedances for compositions included an inductance term. The results of fitting calculations delivered the , , and parameters, the Warburg characteristics (for high temperatures) of samples. All observed impedances were normalized using the dimensions of each pellet (surface and thickness ). As these dimensions were constant for all samples, no correction was necessary.
3. Results
3.1. Phase Identification after Thermal Cycles
In this section, we report a phase identification of typical samples before and after electrical analyses (each sample subjected to three thermal cycles). Let us recall that these identifications were carried out in room conditions, for samples initially elaborated at 600°C and then thermally treated up to 750°C during EIS analyses. Scanning electron microscopy images have been presented and commented in our previous work [1].
Figures 2(a), 2(b), and 2(c), respectively, report the six Xray diffraction patterns for samples (phase ), (phase β), and (phase α) recorded in room conditions before and after EIS cycles. These analyses, performed before and after EIS experiments, clearly show that, after successive thermal treatments, three types of complex stabilized systems are formed and observable at 25°C. For composition , the major phase coexists with traces of monoclinic αBi_{2}O_{3} phase; for composition , the β phase is changed into the phase coexisting with the monoclinic phase; for composition , αBi_{2}O_{3} monoclinic and traces of δBi_{2}O_{3} cubic phase coexist. The presence of this cubic phase in this last sample is probably due to structural quenching during cooling process from 750°C. The presence of traces of monoclinic form in samples and may be interpreted in terms of diffusion of defects from the tetragonal phases.
(a)
(b)
(c)
3.2. Electrical Properties
Figure 3 represents a series of Nyquist plots at 400°C for the 11 samples. Below composition , the plots constitute unique Nyquist circles associated with graincore conduction. Above composition , two circles are observed (associated with grainboundary and graincore conduction) with a linear contribution at low frequency corresponding to conduction and diffusion at the electrodes. This contribution might be assimilated mainly to an ionic conduction corresponding to ionic diffusion along grain boundaries and at the electrode interfaces.
(a)
(b)
(c)
On Figures 4(a) and 4(b), we have represented a series of Nyquist plots at 600, 650, 700, and 750°C for composition .
(a)
(b)
On Figures 5(a), 5(b), 5(c), and 5(d), we have reported a part of the results of modeling calculations, with corresponding equivalent circuits. Figure 5(a) is relative to sample (ceria) with equivalent circuit at 700°C. Figure 5(b) is relative to sample with model at 400°C. Figure 5(c) is relative to sample with equivalent circuit at 300°C. Figure 5(d) is relative to sample with equivalent circuit at 600°C.
(a)
(b)
(c)
(d)
For temperatures °C, the impedance is given by . The results concerning the CPE terms for typical temperatures (300, 350, 400, and 450°C) are reported in Table 2(a). The resistance values are not reported here (see Figure 6 representing the conductivity versus temperature and composition). The values increase as composition (or temperature ) increases, and the values determined at low temperatures (°C) decrease from 0.9 and 0.8 as temperature increases.
(a)  
 
(b)  
 
(c)  

In the high temperature range (°C), the values can be described from several electrical components including an inductance . The general value has been expressed using three components as follows: . The term should represent external electrical terminals (metallic junctions) mixed with a main sample contribution (grain core): as depends on composition and temperature, it cannot be linked to such metallic contributions. The term has a CPE form and can be linked to sample interfaces: . The term should represent the electrode contribution. We have observed that a typical modified Warburg form could better describe the Nyquist curves ( contribution). It is the reason why we did not use the usual CPE form. As the , , and values strongly decrease with temperature, we have considered that they were mainly associated with sample and/or interface evolutions including electrodesample interfaces. The sample resistance was determined as being the sole term representing the bulk properties.
In Table 2(b), we have reported a series of results concerning a typical sample at composition and for various temperatures. This table is decomposed into three sections corresponding to three temperature ranges: °C ( component), °C (), °C ().
The values associated with grain cores (sample ) increase as a function of temperature. The values decrease from to . The thermal variations of the characteristics (), and () are related to the thermal evolutions of heterogeneous grain boundaries and heterogeneous electrodematerial junctions.
The values decrease (from 0.7 to 0.5) and the values increase as a function of temperature, between 300 and 450°C. The , and values decrease as temperature increases. The mean values are close to 0.65. The values are close to 0.3. These low values of exponents validate the existence of diffusional process linked to ionic conduction. The values of increase with temperature, while the term seems to irregularly vary.
In Table 2(c), we have reported partial results concerning a series of samples (variable composition ) at a fixed temperature of 700°C. In the composition range , the impedance model is . Above , the impedance model is expressed as being .
At this high temperature, electrical evolutions are described through the following typical fitting parameters:(i)the values (grain core) reach a minimum for compositions close to ;(ii)the values (electrodesample interface) vary in an irregular way;(iii)the values (electrodesample interface) increase with ;(iv)the values irregularly vary close to a mean value of 0.5;(v)the resistances decrease with composition ;(vi)the values (Warburg diffusion component) increase with ;(vii) the values irregularly vary close to the mean value of 0.35.
It should be remarked that the exponent is close to 0.5, while the exponent is less than 0.5 (expected theoretical Warburg value).
Figure 6 gives the values of the logarithm of conductivity log(σ) as a function of the composition and for temperatures ranging between 400 and 750°C. The σ values were determined from the values and sample dimensions. Table 3 gives the values of the activation energies as a function of composition and for various temperature ranges. At low temperatures, low values of activation energies due to extrinsic defects are observed (close to eV). In the temperature range °C and for compositions , the activation energy first decreases from to 1.09 eV then increases up to 1.19 eV. For compositions .5, we observe a modification in activation energy above 500°C: in the temperature range °C, this activation energy is of about 1.35 eV while between 500 and 750°C, it decreases to a value of 1.0 eV. This modification might be related to a change in charge carriers with probably a significant contribution of ionic conduction.

Finally, the observed increasing conductivity as increases should have two complementary origins: increasing charge carriers due to Bi^{3+} and vacancies increasing fractions, and lattice energy softening due to Bi–O bonds (the activation energy being closely related to the lattice energy). This type of effect was previously suggested by Mandal et al. [43].
4. Discussion
The values of apparent conductivities, presently determined in our specific conditions, depend on experimental parameters, for example, compaction pressure, porosity, and grain sizes. These values are weaker than the values obtained by Hull et al. [28] for samples sintered at various temperatures ranging between 900 and 1300°C and corresponding to compositions (solid solution). This can be easily explained first by the fact that our samples were initially sintered at 600°C then heated up to 750°C during electrical measurements and secondly by the fact that they present a certain degree of porosity (see Table 1). In the case of mix systems with high values, it is not possible to exceed the fusion temperature of Bi_{2}O_{3} (°C) while this is fully acceptable in the case of solid solutions for low values.
In the composition range , the log(σ) values (Figure 5) increase with composition . For these samples, the nature of conduction is probably electronic and ionic. The ionic contribution can be directly attributed to the increasing number of structural defects Bi^{3+}Bi^{3+} that can offer a great number of diffusion paths for oxygen ions through the oxygen vacancies □.
In the composition range , we have observed a new evolution with a maximum of conductivity at . This evolution might be clearly ascribed to the existence of a biphasic solidsolution system based on a solid solution having a ceria structure with disordered Bi^{3+} and vacancy defects, coexisting with a tetragonal Bi_{2}O_{3} lattice that probably has cerium defects. As the proportion of the highly conducting Bi_{2}O_{3} phase increases, the ionic conduction also increases. For compositions greater than , the conductivity decreases. Two effects are in competition in these conductivity values: the high ionic conduction of the bismuth phase and the microstructure of the samples. As shown in our previous work [1], the specific surface areas exhibit a strong variation as increases. In the solidsolution range , the BET analyses showed that specific surface areas are very high, whereas the specific surface areas strongly decrease as increases in the biphasic system due to crystal growth of the bismuth phase. Thus, this evolving microstructure in the compacted pellets could play a prominent role in conduction. Cavities may play a decisive role in ionic conduction due to the formation of the tetragonal β phase.
Finally, in the case of the monoclinic Bi_{2}O_{3} phase obtained for , the observed large conductivity decrease can be attributed to the more compact monoclinic structure compared to the previous tetragonal ones, which limits oxygen mobility. For this monoclinic Bi_{2}O_{3} phase, we have observed the expected transition [20, 23, 24] at °C, with a large increase in conductivity due to the structural transformation involving a specific volume increase (monoclinic phase transforming into the cubic phase).
5. Conclusions
In this CeO_{2}Bi_{2}O_{3} system produced at 600°C under air, the main result should reside in the high conductivity of the polycrystalline and compacted mix system with compositions close to 0.60.7. In this composition range, the stabilization of the tetragonal phase should be responsible for such a high conductivity. In our EIS experiments, this complex system is stabilized after two thermal cycles. In the composition range , we observe a large increase in conductivity mainly due to ionic conduction of oxygen ions in this tetragonal Bi_{2}O_{3} lattice. This ionic conduction is clearly suggested by the Warburg components in Nyquist representations (for °C). For compositions , a new tetragonal structure βBi_{2}O_{3} is formed at 600°C: however, it evolves after thermal treatment and gives rise to a more complex system where and α phases coexist. This modification of the β phase into and α phases might be ascribed to thermal cycling up to 750°C involving ionic diffusion: this should argue in favor of a higher stability of the phase due to a sufficiently proportion of cerium ions in the tetragonal lattice. For , the monoclinic αBi_{2}O_{3} phase systematically presents a conductivity lower than the one of the mix system with composition .
Finally, the mix system with composition close to should be an interesting optimized electrolyte for applications limited to temperatures of 700°C: below this temperature, the stability of the system should be ensured.
Appendix
According to authors of [39–43], the Warburg element can be expressed as follows: where is a pulsation and is equal to 1/2. In this expression, is related to the chemical diffusion constant (in m2·s1), , is a length characteristic of reaction process. The term has the dimension of a resistance (in Ω). In the case of heterogeneous interfaces, the exponent can be different from . This model could account for ionic diffusion associated with gas formation at grain boundaries and electrode interfaces: O2 ↔ 2e + (1/2)O2 (g).
Acknowledgments
The authors gratefully acknowledge the ProvenceAlpesCôte d’Azur Regional Council, the General Council of Var, and the agglomeration community of Toulon Provence Mediterranean for their helpful financial supports. This work was developed in the general framework of ARCUS CERES project (2008–2010).
References
 L. Bourja, B. Bakiz, A. Benlhachemi et al., “Structural, microstructural and surface properties of a specific CeO_{2}Bi_{2}O_{3} multiphase system obtained at ${600}^{\xb0}$C,” Journal of Solid State Chemistry, vol. 184, no. 3, pp. 608–614, 2011. View at: Publisher Site  Google Scholar
 J. Kašpar, P. Fornasiero, and M. Graziani, “Use of CeO_{2}based oxides in the threeway catalysis,” Catalysis Today, vol. 50, no. 2, pp. 285–298, 1999. View at: Google Scholar
 A. Trovarelli, “Catalytic properties of ceria and CeO_{2}containing materials,” Catalysis Reviews, vol. 38, no. 4, pp. 439–520, 1996. View at: Google Scholar
 A. Trovarelli, C. Leitenburg, M. Boaro, and G. Dolcetti, “The utilization of ceria in industrial catalysis,” Catalysis Today, vol. 50, no. 2, pp. 353–367, 1999. View at: Google Scholar
 A. Tschope, W. Liu, M. F. Stephanopoulos, and J. Y. Ying, “Redox activity of nonstoichiometric cerium oxidebased nanocrystalline catalysts,” Journal of Catalysis, vol. 157, no. 1, pp. 42–50, 1995. View at: Publisher Site  Google Scholar
 T. Masui, K. Minami, K. Koyabu, and N. Imanaka, “Synthesis and characterization of new promoters based on CeO_{2}ZrO_{2}Bi_{2}O_{3} for automotive exhaust catalysts,” Catalysis Today, vol. 117, no. 1–3, pp. 187–192, 2006. View at: Publisher Site  Google Scholar
 X. Zheng, X. Zhang, Z. Fang, X. Wang, S. Wang, and S. Wu, “Characterization and catalysis studies of CuO/CeO_{2} model catalysts,” Catalysis Communications, vol. 7, no. 9, pp. 701–704, 2006. View at: Publisher Site  Google Scholar
 O. Demoulin, M. Navez, J.L. Mugabo, and P. Ruiz, “The oxidizing role of CO_{2} at mild temperature on ceriabased catalysts,” Applied Catalysis B, vol. 70, no. 14, pp. 284–293, 2007. View at: Publisher Site  Google Scholar
 E. Aneggi, M. Boaro, C. D. Leitenburg, G. Dolcetti, and A. Trovarelli, “Insights into the redox properties of ceriabased oxides and their implications in catalysis,” Journal of Alloys and Compounds, vol. 408412, pp. 1096–1102, 2006. View at: Publisher Site  Google Scholar
 M. Mogensen, N. M. Sammes, and G. A. Tompsett, “Physical, chemical and electrochemical properties of pure and doped ceria,” Solid State Ionics, vol. 129, no. 1, pp. 63–94, 2000. View at: Publisher Site  Google Scholar
 R. N. Blumenthal and R. K. Sharma, “Electronic conductivity in nonstoichiometric cerium dioxide,” Journal of Solid State Chemistry, vol. 13, no. 4, pp. 360–364, 1975. View at: Google Scholar
 L. Aneflous, J. A. Musso, S. Villain, J. R. Gavarri, and H. Benyaich, “Effects of temperature and Nd composition on nonlinear transport properties in substituted Ce_{1x}Nd_{x}O_{2δ} cerium dioxides,” Journal of Solid State Chemistry, vol. 177, no. 3, pp. 856–865, 2004. View at: Publisher Site  Google Scholar
 P. Shuk, M. Greenblatt, and M. Croft, “Hydrothermal synthesis and properties of Ce_{1x}EuxO_{2δ} solid solutions,” Journal of Alloys and Compounds, vol. 303304, pp. 465–471, 2000. View at: Google Scholar
 B. Matovic, Z. DohcevicMitrovic, M. Radovic et al., “Synthesis and characterization of ceria based nanometric powders,” Journal of Power Sources, vol. 193, no. 1, pp. 146–149, 2009. View at: Publisher Site  Google Scholar
 R. O. Fuentes and R. T. Baker, “Synthesis and properties of Gadoliniumdoped ceria solid solutions for ITSOFC electrolytes,” International Journal of Hydrogen Energy, vol. 33, no. 13, pp. 3480–3484, 2008. View at: Publisher Site  Google Scholar
 P. Jasinski, “Electrical properties of nanocrystalline Smdoped ceria ceramics,” Solid State Ionics, vol. 177, no. 26–32, pp. 2509–2512, 2006. View at: Publisher Site  Google Scholar
 P. Shuk, M. Greenblatt, and M. Croft, “Hydrothermal synthesis and properties of mixed conducting Ce_{1x}TbxO_{2δ} solid solutions,” Chemistry of Materials, vol. 11, no. 2, pp. 473–479, 1999. View at: Google Scholar
 L. G. Sillen, Arkiv for Kemi, Mineralogi Och Geologi, vol. 12A, 1937.
 V. Fruth, A. Ianculescu, D. Berger et al., “Synthesis, structure and properties of doped Bi_{2}O_{3},” Journal of the European Ceramic Society, vol. 26, no. 14, pp. 3011–3016, 2006. View at: Publisher Site  Google Scholar
 N. M. Sammes, G. A. Tompsett, H. Näfe, and F. Aldinger, “Bismuth based oxide electrolytes—structure and ionic conductivity,” Journal of the European Ceramic Society, vol. 19, no. 10, pp. 1801–1826, 1999. View at: Google Scholar
 L. E. Depero and L. Sangaletti, “Structural disorder and ionic conduction: the case of Bi_{2}O_{3},” Journal of Solid State Chemistry, vol. 122, no. 2, pp. 439–443, 1996. View at: Publisher Site  Google Scholar
 C. N. R. Rao, G. V. S. Rao, and S. Ramdas, “Phase transformations and electrical properties of bismuth sesquioxide,” The Journal of Physical Chemistry, vol. 73, no. 3, pp. 672–675, 1969. View at: Publisher Site  Google Scholar
 H. A. Harwig and A. G. Gerards, “Electrical properties of the α, β, γ, and δ phases of bismuth sesquioxide,” Journal of Solid State Chemistry, vol. 26, no. 3, pp. 265–274, 1978. View at: Google Scholar
 P. Shuk, H.D. Wiemhöfer, U. Guth, W. Göpel, and M. Greenblatt, “Oxide ion conducting solid electrolytes based on Bi_{2}O_{3},” Solid State Ionics, vol. 89, no. 34, pp. 179–196, 1996. View at: Google Scholar
 O. Monnereau, L. Tortet, P. L. lewellyn, F. Rouquerol, and G. Vacquier, “Synthesis of Bi_{2}O_{3} by controlled transformation rate thermal analysis: a new route for this oxide?” Solid State Ionics, vol. 157, no. 1–4, pp. 163–169, 2003. View at: Publisher Site  Google Scholar
 F. Schröder and N. Bagdassarov, “Phase transitions and electrical properties of Bi_{2}O_{3} up to 2.5 GPa,” Solid State Communications, vol. 147, no. 910, pp. 374–376, 2008. View at: Publisher Site  Google Scholar
 F. Schröder, N. Bagdassarov, F. Ritter, and L. Bayarjargal, “Temperature dependence of Bi_{2}O_{3} structural parameters close to the α δ pphase transition,” Phase Transitions, vol. 83, no. 5, pp. 311–325, 2010. View at: Publisher Site  Google Scholar
 S. Hull, S. T. Norberg, M. Tucker, S. Eriksson, C. Mohn, and S. Stølen, “Neutron total scattering study of the δ and β phases of Bi_{2}O_{3},” Dalton Transactions, no. 40, pp. 8737–8745, 2009. View at: Publisher Site  Google Scholar
 S. Dikmen, P. Shuk, and M. Greenblatt, “Hydrothermal synthesis and properties of Ce_{1x}BixO_{2δ}solid solutions,” Solid State Ionics, vol. 112, no. 34, pp. 299–307, 1998. View at: Google Scholar
 X. L. Chen and W. Eysel, “The stabilization of βBi_{2}O_{3} by CeO_{2},” Journal of Solid State Chemistry, vol. 127, no. 1, pp. 128–130, 1996. View at: Publisher Site  Google Scholar
 K. Sardar, H. Y. Playford, R. J. Darton et al., “Nanocrystalline ceriumbismuth oxides: synthesis, structural characterization, and redox properties,” Chemistry of Materials, vol. 22, no. 22, pp. 6191–6201, 2010. View at: Publisher Site  Google Scholar
 M. J. Godinho, R. F. Gonçalves, L. P. S Santos, J. A. Varela, E. Longo, and E. R. Leite, “Room temperature coprecipitation of nanocrystalline CeO_{2} and Ce_{0.8}Gd_{0.2}O_{1.9δ} powder,” Materials Letters, vol. 61, no. 89, pp. 1904–1907, 2007. View at: Publisher Site  Google Scholar
 J. G. Li, T. Ikegami, Y. Wang, and T. Mori, “Nanocrystalline Ce_{1x}Y_{x}O_{2x/2} ($0\le x\le 0.35$) oxides via carbonate precipitation: synthesis and characterization,” Journal of Solid State Chemistry, vol. 168, no. 1, pp. 52–59, 2002. View at: Publisher Site  Google Scholar
 F. Ye, T. Mori, D. R. Ou, J. Zou, and J. Drennan, “Microstructural characterization of terbiumdoped ceria,” Materials Research Bulletin, vol. 42, no. 5, pp. 943–949, 2007. View at: Publisher Site  Google Scholar
 Y. Ikuma, K. Takao, M. Kamiya, and E. Shimada, “Xray study of cerium oxide doped with gadolinium oxide fired at low temperatures,” Materials Science and Engineering B, vol. 99, no. 1–3, pp. 48–51, 2003. View at: Publisher Site  Google Scholar
 Y. P. Fu and S. H. Chen, “Preparation and characterization of neodymiumdoped ceria electrolyte materials for solid oxide fuel cells,” Ceramics International, vol. 36, no. 2, pp. 483–490, 2010. View at: Publisher Site  Google Scholar
 D. Johnson, Zview, Impedance software, Version 2.1a, Scribner Associates Inc, (1990–1998).
 J. R. Macdonald, “Double layer capacitance and relaxation in electrolytes and solids,” Transactions of the Faraday Society, vol. 66, pp. 943–958, 1970. View at: Publisher Site  Google Scholar
 J. R. Macdonald, “Electrical response of materials containing space charge with discharge at the electrodes,” The Journal of Chemical Physics, vol. 54, no. 5, pp. 2026–2050, 1972, Erratum: electrical response of materials containing space charge with discharge at the electrodes, The Journal of Chemical Physics, vol. 56, article, 681, 1972. View at: Google Scholar
 J. R. Macdonald, “Impedance spectroscopy: old problems and new developments,” Electrochimica Acta, vol. 35, no. 10, pp. 1483–1492, 1990. View at: Google Scholar
 J. R. Macdonald, “Characterization of the electrical response of high resistivity ionic and dielectric solid materials by immittance spectroscopy,” in Impedance Spectroscopy—Theory, Experiment, and Applications, E. Barsoukov and J. R. Macdonald, Eds., pp. 264–282, John Wiley & Sons, New Jersey, NJ, USA, 2nd edition, 2005. View at: Google Scholar
 C. Ho, I. D. Raistrick, and R. A. Huggins, “Application of AC techniques to the study of lithium diffusion in tungsten trioxide thin film,” Journal of the Electrochemical Society, vol. 127, no. 2, pp. 343–349, 1980. View at: Google Scholar
 B. P. Mandal, S. K. Deshpande, and A. K. Tyagi, “Ionic conductivity enhancement in Gd_{2}Zr_{2}O_{7} pyrochlore by Nd doping,” Journal of Materials Research, vol. 23, no. 4, pp. 911–916, 2008. View at: Publisher Site  Google Scholar
Copyright
Copyright © 2012 Lamia Bourja et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.